Properties of Stabilized Peat by Soil-Cement Column ... - Ejge.com
Vol. 13, Bund. J 4 Field experiment Soil-cement column (height 1000 mm and diameter 200 mm.) were constructed by using ordinary Portland cement, bentonite, calcium chloride as binder. Dosage rate of binder was 300 kg/m 3 . Mixing proportion of binder was 1) YTL Cement and bentonite in 85:15 ratio and 25% 0f well graded sand by volume of soil 2) 100 % of Mascrete (Lafarge brand) cement, CaCl 2 (4 % of binder) and 25% of sand by volume of soil. Column was conducted by premixed and premixed method in which a 200 mm diameter and 1000 mm height whole was made by drilling a hand operated auger. Soil and binder were mixed in a tray and the mixer was inserted into the whole. Hand operated cone penetrometer A proving ring hand operated cone penetrometer has been used in this experiment which consists of a T handle, penetration rod, proving ring of 1 kN capacity with dial indicator, and a removable cone point. The penetrometer is pressed into the soil manually and relates the force required to drive the probe a certain distance through a soil in order to determine the relative density, stiffness, strength or bearing capacity (Cernica, 1995). Unconfined compression test Sample was collected from stabilised column to conduct unconfined compressive strength test (UCT) in laboratory. The test was performed in a 50 mm diameter and 100-mm height mould according to BS 1377:1990. Direct shear box test 60 mm x 60 mm x 300 mm column have been formed in field using cement, CaCl2 and silica sand as binder. After 14 days of curing the column have been collected and brought to laboratory and performed direct shear box test to know shear strength for different normal stress condition . The test was conducted by following BS 1377:1990. RESULT AND DISCUSSION Observation of visual inspection The columns have been exposed after 14 days of curing period and it was found that a 200 mm diameter circular shape uniform column has formed. There is an effect of stabilising agent in surrounding soils and the effect was in between 10 mm to 30 mm from the outer edge of columns. There will be a mechanical interaction in between column and surrounding soils and applied load can be carried out by both, which was indicated in design consideration of EuroSoilStab, 2002. Plate 1 shows the formation of column both in horizontal and vertical direction.
Undrained shear strength (MPa) Vol. 13, Bund. J 5 Plate 1: a) Formation of column after 14 days b) vertically exposed column Effect on undrained shear strength From the cone penetrometer test it was observed that undrained shear strength has reached at 1.60 Mpa (Fig. 1) for the column stabilised by the mix design with cement, CaCl2 and sand. Binding agent of cement, bentonite and sand had a considerable effect on undrained shear strength which was 0.86 Mpa. This result seems to be higher because the result of cone penetrometer sometime misleads but nevertheless this result indicated that the bearing capacity of stabilised column increased dramatically after stabilisation. 1.60 1.40 1.20 1.00 0.80 0.60 0.40 0.20 0.00 0 5 10 15 20 25 Curing period (Days) Lafarge cement (100% of binder) + CaCl2 (4% of binder) + Sand (25% of wet peat in volume basis) Figure 1: Undrained shear strength of stabilised column after 14 days curing time